Supplementary materials surface species on SiO2 precursors ...
Embed Size (px)
Transcript of Supplementary materials surface species on SiO2 precursors ...
Ethoxy and silsesquioxane derivatives of antimony as dopant precursors: unravelling the structure and thermal stability of
surface species on SiO2
T. Alphazan,a,b P. Florianc and C. Thieuleuxb,*
a. Univ. Grenoble Alpes, FR-38000 Grenoble, CEA, LETI, Minatec Campus, FR-38054 Grenoble Cedex 9, France
b. C2P2, CPE Lyon, 43 Bd du 11 Nov. 1918, 69616 Villeurbanne cedex France
c. Conditions Extrêmes et Matériaux: Haute Température et Irradiation, CNRS-UPR 3079, 1 d Avenue de la Recherche Scientifique, 45071 Orléans, Cedex 2, France
OutlineSI 1. General procedures and methods ..................................................................................2
SI 2. DSC analysis of POSS-triol, POSS-P and POSS-Sb.....................................................8
SI 3. TGA analysis of POSS-triol, POSS-P and POSS-Sb .....................................................9
SI 4. Thermal stability of molecular POSS-Sb followed by in-situ IR ....................................10
SI 5. 29Si CPMAS NMR spectra of SiO2 -supported POSS-Sb materials..............................11
SI 6: Differential IR spectra of SiO2 supported POSS-Sb materials......................................12
SI 7. IR (DRIFT) spectra of 18O-doped SiO2-(700) and related Sb-material .............................13
SI 8. 1H MAS and 13C CPMAS NMR spectra of [Sb(OEt)3]2/SiO2-(500) ...................................14
SI 9. 121Sb NMR spectra of POSS-Sb and [Sb(OEt)3]2..........................................................15
SI 10. Decomposition of [Sb(OEt)3]2/SiO2-(500) followed by in-situ IR-GC/MS........................17
SI 11. References .................................................................................................................20
Electronic Supplementary Material (ESI) for Physical Chemistry Chemical Physics.This journal is © the Owner Societies 2017
SI 1. General procedures and methods
All experiments, otherwise stated, were carried out under dry and oxygen free Ar
atmosphere using either standard Schlenk or glovebox (GB) techniques for the organic
synthesis. For syntheses and treatments of surface species, reactions were carried out
using high vacuum lines (10-5 mbar). Elemental analyses of supported materials were
performed at “Mikroanalytisches Labor Pascher” in Germany. High resolution mass
spectroscopy (HR-MS) was performed with a micrOTOF-Q II from Bruker, in ESI+ mode.
Toluene and pentane were dried using an MBraun solvent purification system, contacted
with molecular sieves 4 Å and degassed under vacuum. Hepta-isobutyl-POSS triol
(POSS-OH), antimony(III) chloride (SbCl3), antimony(III) ethoxide ([Sb(OEt)3]2) and
triethylamine (Et3N) were purchased from Sigma Aldrich. Et3N was distilled over CaH2
prior to use. [Sb(OEt)3]2 was distilled under reduced pressure to give a colourless,
moisture sensitive liquid stored in the glovebox.
FTIR and in-situ FTIR coupled with GC/MS. FTIR spectra recorded in diffuse reflectance
infrared Fourier transform spectroscopy (DRIFT) mode were obtained on a Nicolet 6700
FT-IR spectrometer equipped with a HgCdTe (MCT) detector cooled with liquid N2. The
samples were loaded into a custom DRIFT cell equipped with CaF2 windows (or ZnSe
for in-situ experiments) under inert atmosphere (glovebox). Typically, 64 scans were
acquired (4 cm-1 resolution). For in-situ experiments, 4 spectra per minute were acquired
in average; materials were decomposed under a flux (10 ml.min-1) of dry gas (air or N2),
with a heating rate of 6°C.min-1, from ~20°C to 500°C (or 650°C), and maintained at the
desired temperature before being cooled. Gases, released during thermal treatment,
were collected and analyzed by GC/MS for identification.
Liquid state NMR. Liquid-state NMR spectra were recorded using a Bruker Spectrospin
300 MHz spectrometer. 1H, 13C and chemical shifts were referenced to TMS at 0 ppm.
Solid-state NMR. 40 to 50 mg of material was packed in 4.0 mm zirconia NMR rotor
under inert atmosphere. NMR spectra were acquired either on a 300 MHz or 500 MHz
ultrashieldedBruker NMR spectrometer.1H, 13C and 29Si spectra were recorded using a
4.0 mm cross-polarization (CP) magic angle spinning (MAS) probe with a sample
temperature of 294 K and sample spinning frequencies between 5 to 10 kHz. Standard
CP was used to record 29Si and 13C spectra. 1H, 13C and chemical shifts were
referenced to TMS at 0 ppm. 121Sb NMR spectra were obtained on a Bruker Avance III
850 spectrometer operating at 20.0T (203.5MHz for 121Sb) and using a “low-gamma”
4mm MAS probe under static conditions with radio-frequency fields of 80kHz.
Thermogravimetric analysis (TGA).TGA experiments were performed on a Mettler
DSC/TGA StarSyst apparatus. 10 mg of material were loaded in a sealed aluminium pan
under inert atmosphere. Analyses were performed under a flux (10 ml.min-1) of gas (air,
N2), from ~20°C to 500°C (6°C.min-1), then at 500°C (isotherm) for 90 min.
Differential scanning calorimetry (DSC). DSC experiments were performed on a Mettler
DSC 2 StarSyst apparatus, using the same parameters as for TGA.
Synthesis of hepta-isobutyl-polyhedral oligomeric silsesquioxane antimony triester
(POSS-Sb). POSS-Sb was prepared as described in the main text. Yield: 55% (1.42 g).
1H NMR, 13C NMR and 29Si NMR: see main text. 121Sb NMR (ppm): very broad signal.
HR-MS: m/z [M+H]+= 909.1803 (expected for C28H64O12Si7Sb: 909.1815). XRD:
Monocrystals were grown by slow evaporation of a toluene solution, or at low
temperature (-30 °C) in GB. However, no structure resolution was possible.
Antimony(III) ethoxide. Commercial Sb(OEt)3 [sigma] was a redish liquid. Distillation
under a slightly reduced pressure (Schlenk line) at about 70°C gave a colorless liquid,
highly moisture and O2 sensitive, that was stored in GB. 1H NMR (C6D6, 25 °C, ppm):
δH= 4.02 (q, 2H, CH2CH3), 1.23 (t, 3H, CH2CH3).13C NMR (ppm): δC= 58.9 (CH2CH3),
20.2 (CH2CH3). IR (cm-1): 2967, 2921, 2866 ν(C-H); 2746, 2715 (s, 2xδ(C-H)); 2610
(vw); 1925 (vw); 1477, 1442, 1380, 1359 δ(C-H);1284 (vw), 1155, 1094 C-H; 1041
νas(CCO); 891 νs(CCO); 805 (vw); 550 (broad) v(Sb-O)1,2
Study on silica nanoparticles (NPs).
Preparation of partially dehydroxylated silica at 700 °C (SiO2-(700)). Silica powder (see
main text) was calcined for 5 h under air at 500 °C (6 °C.min-1), partially dehydroxylated
at 500°C in secondary vacuum (10-5 mbar) for 12 h, then at 700 °C for 10 h, and finally
stored in the glovebox. SBET (m².g-1): 197. IR (cm-1): 3747 (isolated SiOH), 3600 (large
peak, very low intensity, bonded SiOH).
Quantification of surface SiOH groups (OH.nm-2) found onto SiO2. The procedure was
Preparation of 18O-doped SiO2-(700). The procedure, using a vapor pressure of H218O and
SiO2-(700), was described elsewhere.4
Grafting POSS-Sb onto SiO2-(500). Representative procedure. POSS-Sb (468 mg, 5.1 x
10-4 mol, 0.7 eq) was solubilized in pentane (10 mL) and was subsequently contacted
with SiO2-(500) (~1.0 g, ~7.3 x 10-4 mol surface silanol) at 25 °C for 2.5 h, under gentle
stirring. After filtration, the solid was washed 3 times with pentane, and all volatile
compounds were removed in vacuo (10-3 mbar). The resulting solid POSS-Sb/SiO2-(500)
was dried under high vacuum (10-5 mbar) and the grafted species were then stored
under Argon. IR (cm-1): 3746 (remaining isolated SiOH), 3702 (perturbed, H-bonded
SiOH), 3364 (broad), 2960, 2933, 2908 & 2875 ν(C-H), 2782, 2724, 2629 (probable
combination bands or overtones of CH groups), 1468 & 1403 δ(C-H). 1H MAS NMR
(ppm): δH= 1.8 (CH2CH(CH3)2), 0.9 (CH2CH(CH3)2 and CH2CH(CH3)2). 13C NMR (CP-
MAS, ppm): δC= 24 (broad). 29Si NMR (HP-Dec, ppm): δSi= –57 (~1 Si, T2-SiOH, POSS
cage), –66 (6 Si, T3-type, POSS cage), ca. –108 (broad, Q-type Si, SiO2 network).
Elemental analysis: 3.16 wt % C, 0.60 wt % H, 1.09 wt % Sb, i.e. H/C(at/at)= 2.3,
C/Sb= 29.4 and 0.27 Sb/nm² corresponding to ~14% grafting. Expected for (Si-
O)SbC28H64O12Si7: H/C(at/at)= 2.3, C/Sb= 28.0. Misc: Only pure POSS-Sb was
recovered from the solution after grafting/rinsing.
Grafting POSS-Sb onto SiO2-(700)18O-doped. POSS-Sb/Si18O2-(700) was prepared
according to the representative procedure, with 215 mg of Si18O2-(700) (~5.0 × 10-5 mol
surface silanols) and 52 mg of POSS-Sb (5.7 × 10-5 mol, 1.1 eq). IR (cm-1): 3745
(remaining isolated Si16OH), 3734 (remaining isolated Si18OH), 3699 (perturbed, H-
bonded SiOH), 3363 (broad), 2960, 2933, 2908 & 2875 ν(C-H), 2782, 2724, 2629
(probable combination bands or overtones of CH groups), 1468 δ(C-H).
Grafting POSS-Sb onto SiO2-(140). POSS-Sb/SiO2-(140) was prepared according to the
representative procedure, with 330 mg of SiO2-(140) (~5.0 × 10-4 mol surface silanols) and
206 mg of POSS-Sb (2.3 × 10-4 mol, 0.5 eq). IR (cm-1): 3741 (remaining isolated SiOH),
3696 (perturbed, H-bonded SiOH), 3450 (broad), 2958, 2943, 2906 & 2875 ν(C-H),
2782, 2728, 2628 (probable combination bands or overtones of CH groups), 1468 δ(C-
H). 1H MAS NMR (ppm): δH= 1.9 (CH2CH(CH3)2), 0.9 (CH2CH(CH3)2 and CH2CH(CH3)2).
13C NMR (CP-MAS, ppm): δC= 24 (broad). 29Si NMR (HP-Dec, ppm): δSi= –57 (~2.5 Si,
T2-SiOH, POSS cage), –66 (T3-type, POSS cage), ca. –109 (broad, Q-type Si, SiO2
network). Elemental analysis: 4.20 wt % C, 0.88 wt % H, 1.53 wt % Sb, i.e. H/C(at/at)=
2.5, C/Sb= 28.0 and 0.38 Sb/nm² corresponding to ~9% grafting. Expected for (Si-
O)2SbC28H65O12Si7: H/C(at/at)= 2.3, C/Sb= 28.0. Misc: Only pure POSS-Sb was
recovered from the solution after grafting/rinsing.
Grafting [Sb(OEt)3]2 onto SiO2-(500). [Sb(OEt)3]2/SiO2-(500) was prepared according to the
representative procedure, with ~120 µl (~7.1 x 10-4 mol, 1.2 eq) of [Sb(OEt)3]2 and 766
mg of SiO2-(500) (~5.6 x 10-4 mol surface silanol) at 25 °C. IR (cm-1): 3664 (perturbed, H-
bonded SiOH), 2972, 2929, 2889 & 2875 ν(C-H), 2752, 2723, 2704 (probable
combination bands or overtones of CH groups), 2614 (already observed in the starting
compound), 1478, 1445 & 1385 δ(C-H). 1H MAS NMR (ppm): δH= 3.9 (CH2CH3), 1.1
(CH2CH3). 13C NMR (CP-MAS, ppm): δC= 58 (CH2CH3), 17 (CH2CH3). Elemental
analysis: 2.78 wt % C, 0.56 wt % H, 7.21 wt % Sb, i.e. H/C(at/at)= 2.4, C/Sb= 3.9 and
1.8 Sb/nm² corresponding to ~90% grafting. Expected for (Si-O)Sb(OEt)2: H/C(at/at)=
2.5, C/Sb= 4.0.
SI 2. DSC analysis of POSS-triol, POSS-P and POSS-Sb
0 100 200 300 400 500
Figure S2: DSC traces of POSS-triol, POSS-P and POSS-Sb under nitrogen, between
30°C and 500°C, 6°C/min.
In our conditions, DSC analyses performed in N2 reveal that the starting POSS cage
melts at 198°C (-32.3 kJ/mol) while POSS-Sb and POSS-P melt at 136°C (-32.9 kJ/mol)
and 122°C (-21.5 kJ/mol), respectively
SI 3. TGA analysis of POSS-triol, POSS-P and POSS-Sb
0 100 200 300 400 500
A Under N2 B Under air
0 100 200 300 400 500
Temperature (°C) Temperature (°C)
Figure S3: TGA traces of POSS-triol, POSS-P and POSS-Sb under nitrogen (A) and
under air (B), between ~30°C and 500°C (90 min at 500°C), 6°C/min.
SI 4. Thermal stability of molecular POSS-Sb followed by in-situ IR
General comments: due to melting of POSS-Sb, IR (DRIFT) spectra of poor quality
were obtained above 150°C and more. Experiments were performed up to 650°C under
N2, and 500°C under air, due to apparatus specifications. Only spectra recorded at
~20°C, before and after thermal treatment, are provided in the main manuscript.
SI 5.29Si CPMAS NMR spectra of SiO2 -supported POSS-Sb materials
0 - 50 - 100 - 150
Q-type Si of SiO2
T3-type Si of POSS
T2-type SiO-Hof POSS
Figure S5: 29Si CPMAS NMR spectra of SiO2 -supported POSS-Sb materials obtained at
11.7 T, with ωrot/2π = 5 KHz, 45 k scans, a recycle delay of 5 s, and a contact time of 2
ms. * denotes spinning side bands.
SI 6: Differential IR spectra of SiO2 supported POSS-Sb materials
1500 2000 2500 3000 3500
Δν = 95 cm-1
Figure S6: Differential IR spectra of SiO2 supported POSS-Sb materials, referenced to
their corresponding silica support, partially dehydroxylated at 500°C or dehydrated at
Negative bands ~3747 cm-1 are assigned to isolated silanol that have been consumed
Positive bands located between 3000-2850 cm-1 and located at 1467 cm-1 are ascribed
to C-H bonds of iBu groups of POSS.
Positive bands observed at 3403 and 3308 cm-1 are tentatively assigned to SiO-H bonds
of T2-type SiOH groups formed on POSS upon grafting of POSS-Sb.
SI 7. IR (DRIFT) spectra of 18O-doped SiO2-(700) and related Sb-material
3000 3200 3400 3600 3800
Figure S7: IR (DRIFT) spectra of 18O-doped SiO2-(700) (a) and the supported POSS-Sb
material (b). Differential IR spectrum, referenced to 18O-doped SiO2-(700) (c).
SI 8.1H MAS and 13C CPMAS NMR spectra of [Sb(OEt)3]2/SiO2-(500)
Figure S8-A: 1H MAS NMR spectrum of [Sb(OEt)3]2/SiO2-(500) obtained at 11.7 T, with
ωrot/2π = 10 KHz, 8 scans, and recycle delay of 5 s
Figure S8-B: 13C CPMAS NMR spectrum of [Sb(OEt)3]2/SiO2-(500), obtained at 11.7 T,
with ωrot/2π = 10 KHz, 2 k scans, a recycle delay of 30 s, and a contact time of 2 ms
SI 9. 121Sb NMR spectra of POSS-Sb and [Sb(OEt)3]2
File : e:\#data depart\nmr and ssnmr\alphazan_tgir\sb-poss\22\pdata\1\1r
Figure S9-A:121Sb QCPMG-WURST NMR spectrum of POSS-Sb obtained at 20.0T with
200 k scans, with a recycle delay of 0.3s (i.e. 17 h of acquisition time) and a WURST
shape irradiating over 2MHz.
Figure S9-B:121Sb single-pulse NMR spectrum of (liquid) [Sb(OEt)3]2, obtained at 20.0 T,
with 512 scans, a recycle delay of 0.3 s, and using a 90° pulse at a radio-frequency field
Comments:121Sb is a quadrupolar nuclei, associated with a very large quadrupolar
constant, thus making 121Sb NMR spectra difficult to record (extremely wide line shapes
potentially spreading over several MHz combined with possibly short relaxation times T2)
even for symmetric hexacoordinated compounds such as nearly octahedral KSb(OH)6,
used as reference.5 Here, the large 121Sb signal obtained for the molecular compound
POSS-Sb (2 MHz, Figure S9-A) extends over at least 1.3MHz, i.e. approximately three
times more than the spectra obtained for KSb(OH)6 by Faucher et al. at an equivalent
magnetic field. This result probably originates from the pseudo-trigonal symmetry of the
Sb center in POSS-Sb,6,7 thus increasing Sb quadrupolar constant and broadening the
NMR signal, which –along with a short T2– prevents recording good quality spectra at
room temperature within reasonable acquisition time even using a QCPMG-WURST
acquisition sequence8 (the signal disappeared within the noise in less than 2 ms within
the QCPMG sequence). Besides, 121Sb NMR analysis was intended on [Sb(OEt)3]2 and
confirmed the difficulties to record NMR of quadrupolar nuclei in structure of lower
symmetry..9 Considering these results, we did not try to analyze SiO2-supported
materials as they contain at least 10 times less Sb than molecular compounds and
would require too long acquisition time.
SI 10. Decomposition of [Sb(OEt)3]2/SiO2-(500) followed by in-situ IR-GC/MS
General comments: Experiments were performed up to 650°C under N2, and 500°C
under air, due to apparatus specifications.
2000 2500 3000 3500
500°C Release of ethanal, ethaneand ethene
Release of ethanol
650°C (5 min)
500°C (60 min)
Back to 20°C
(C-H)(O-H) of isolatedand pertubed SiOH
A Under N2
Figure S10-A: IR (in-situ DRIFT) spectra of [Sb(OEt)3]2/SiO2-(500) material, heated from
20°C to 500°C and 650°C (6°C/min), under N2 (10 mL/min).
Comments: The ν(C-H) modes significantly decrease above 400°C, consistent with the
release of several C2 compounds detected by GC/MS. Besides, the similar intensity of
these CH features between 20°C and 350°C suggests that ethanol, released from about
60°C (GC/MS), probably comes from little decomposition of surface species, or traces of
physisorbed EtOH. Note also the appearance, from 500°C, of a band at 3744 cm-1,
which is assigned to isolated SiOH groups, and which thus highlights a modification of
the silica surface, probably linked to the decomposition of surface species. Only
negligible CH bands remains after thermal treatment.
Back to 20°C after 2 h at 500°C
B Under air
2000 2500 3000 3500
(C-H)(O-H) of isolatedand pertubed SiOH
Release of ethanal, thenCO2
Release of ethanol
Figure S10-B: IR (in-situ DRIFT) spectra of [Sb(OEt)3]2/SiO2-(500) material, heated from
20°C to 500°C (6°C/min), under air (10 mL/min).
Comments: The ν(C-H) modes significantly decrease above 200°C, consistent with the
release of ethanal, detected by GC/MS. As for the similar experiment under N2, the
similar intensity of the C-H features between 20°C and 200°C suggests that ethanol,
released from about 60°C (GC/MS), probably comes from little decomposition of surface
species when contacted with air, or traces of physisorbed EtOH. Note also the
appearance of a ν(SiO-H) band (3744 cm-1) assigned to isolated SiOH between 300°C
and 400°C, as well as a ν(C=O) band, consistent with the calcination of organic groups
by O2, and a release of CO2 and H2O. Only negligible CH bands remains after thermal
SI 11. References
1 G. E. Binder, U. Ensinger, W. Dorsch and A. Schmidt, Z. Für Anorg. Allg. Chem., 1983, 507, 163–170.
2 Y. Kawasaki, Y. Yamamoto and M. Wada, Bull. Chem. Soc. Jpn., 1983, 56, 145–148.3 T. Alphazan, L. Mathey, M. Schwarzwälder, T.-H. Lin, A. J. Rossini, R. Wischert, V. Enyedi,
H. Fontaine, M. Veillerot, A. Lesage, L. Emsley, L. Veyre, F. Martin, C. Thieuleux and C. Copéret, Chem. Mater., 2016, 28, 3634–3640.
4 L. Mathey, T. Alphazan, M. Valla, L. Veyre, H. Fontaine, V. Enyedi, K. Yckache, M. Danielou, S. Kerdiles, J. Guerrero, J.-P. Barnes, M. Veillerot, N. Chevalier, D. Mariolle, F. Bertin, C. Durand, M. Berthe, J. Dendooven, F. Martin, C. Thieuleux, B. Grandidier and C. Copéret, J. Phys. Chem. C, 2015, 119, 13750–13757.
5 A. Faucher, V. V. Terskikh and R. E. Wasylishen, Solid State Nucl. Magn. Reson., 2014, 61–62, 54–61.
6 F. J. Feher and T. A. Budzichowski, Organometallics, 1991, 10, 812–815.7 Note: POSS-Sb crystallizes as poorly diffracting crystals from various solvents, thus
preventing any crystal structure resolution. The disorder between isobutyl chains probably explains the poorly diffracting nature of these crystals.
8 L. A. O’Dell and R. W. Schurko, Chem. Phys. Lett., 2008, 464, 97–102.9 J. Autschbach, S. Zheng and R. W. Schurko, Concepts Magn. Reson. Part A, 2010, 36A, 84–